ANSYS, Inc. is an American Computer-aided engineering software developer. Ansys publishes engineering analysis software across a range of disciplines including finite element analysis, structural analysis, computational fluid dynamics, explicit and i
structure influence linesFull description
ANSYS 15.0 ANSYS Explicit Update
Midwest ANSYS Users Group May 18, 2005
Analyzing Hyperelastic Materials w/ Some Practical Considerations Considerations Prepared by: Paris Altidis; Borg Warner Updated by: Vince Adams; IMPACT
Limitations of Hyperelastic Mat’l Models Most material models only allow the analyst to describe only a subset of the structural properties of elastomers. In the Mooney-Rivlin and Ogden formulations: 1. The stress strain functions in the model are stable. They do not change with repetitive loading. The material model does not differentiate between a 1st time strain and a 100 th time straining of the part under analysis. 2. There is no provision to alter the stress strain description in the material model based on the maximum strains experienced. 3. The stress strain function is fully reversible so that increasing strains and decreasing strains use the same stress strain function. Loading and unloading the part under analysis is the same. 4. The models treat the material as perfectly elastic meaning that there is no provision for permanent strain deformation. Zero stress is always zero strain.
Always test your material with loading that is similar to the actual application Contact Axel Products or DatapointLabs for guidelines on what is required. Visit their websites and RTFM (Read Their Fantastic Methods). Many papers can be downloaded for reference. www.axelproducts.com
The recommended method is the ANSYS Curve Fitting Wizard. Hardcore users: Use APDL to create your own scripts for the curve fitting portion and post-processing. For a decent curve fit using the M-R models, you need 2X the number of M-R Parameters. Papers on www.ansys.net provide in-depth info on these techniques… Most will be posted to the MAG site
2-P Mooney-Rivlin vs. Shore Hardness How good is it ? Has been seen in ANSYS and other user groups ONLY For Reference Experience has shown that it is not consistent for ALL GRADES and TYPES of hyperelastic materials. ?
Worth using it in ANSYS as a first pass analysis ?? I’d rather test the material at hand in tension at least. ?
2-P Mooney-Rivlin vs. Shore Hardness E (psi) = 11.427*A -0.4445*A^2 + 0.0071*A^3 Lindemann (XANSYS) From E. F. Gobel, Rubber Springs Design, John Wiley, New York, 1978. 1400 1200 ) I S1000 P ( s u l u 800 d o M s 600 ' g n u o 400 Y
Scope: The performance of an O-Ring (used in a medical device) during assembly as a seal needs to be analyzed and the contact forces to the mating parts be extracted. Element Type: PLANE182 Axisymmetric (Keyopt(1)=0 Full integration with B-bar method (No Hourglass control) Materials: O-Ring: Hyperelastic Material (Other grade information not available); All other parts: Steel
Example of O-Ring Compression Step 1: The lack of information about the material would not allow any guessing (BAD MOVE). So, material tested by Axel products as shown below. Step 2: Curve fitted to 9P M-R Model ( BETTER ) (method APDL)
Elements Supporting Hourglass control : Plane182/183, Solid 164 / 185 / 186 / 45 Use HGSTF Real Constant to Specify the Hourglass stiffness scaling factor However, the artificial energy introduced to control the hourglass effect may affect solution accuracy adversely. Don’t just increase the Stiffness 10% for every successive iteration Bump it up to some high number and then back off Chances are ANSYS will solve FASTER using a HIGH HGSTF rather than a LOW and Gradually increasing value. ?
Wisdom on Hyperelastic Materials from XANSYS - THE School of Hard Knocks ?
For perfectly incompressible material, Poisson’s ratio of 0.5 is unacceptable as it makes the bulk modulus infinite. To keep ANSYS happy, use 0.49995 Polyurethane foams ?? Use Hyper56 with Blatz-Ko function (Keyopt(2)=1) IF you have the parameters for it. The literature is leaning towards M-R or hyperelastic w/ Ogden function. Polyurethane foams and access to LS-DYNA ?? See this reference: http://web.bham.ac.uk/millsnj/pdf/matpaperkyoto.pdf